EFFECT OF RECLAIMED RUBBER CONTENT IN NR/CARBON BLACK VULCANIZATES USING MICROWAVE IRRADIATION SYSTEM C. Kumnuantip* and N. Sombatsompop ** Polymer Processing and Flow (P-PROF) Group, School of Energy and Materials King Mongkut’s University of Technology Thonburi (KMUTT) Bangmod, Bangkok 10140, THAILAND *Also at Faculty of Engineering, Rajamangala Institute of Technology Pathumtani 12120, THAILAND **Corresponding author: email@example.com Abstract This work examined the effect of tire-tread reclaimed rubber content on physical and mechanical properties of natural rubber, vulcanized by microwave (MW) irradiation and thermal cure (CT) systems. The results suggested that the properties of the vulcanizates from CT method was higher than those from MW method except for the swelling level in toluene. The differences in the results between these two curing systems could be explained in terms of the density and the type of crosslinks present in the NR compounds. The microwave cure was more effective as the reclaimed content was increased. Introduction The polymer reclaiming process involves the fracture of higher molecular weight polymer molecules to lower ones . Recent technology to use the reclaimed rubbers in the virgin polymer materials has attracted many rubber industries. Most work in the field have investigated the cure characteristics and the products properties obtained by the incorporation of the reclaimed rubber, in various forms, into different virgin materials (mainly natural rubber). Sombatsompop and Kumnuantip [2-3] introduced tire-tread reclaimed rubber into two natural rubber grades and investigated various properties of the blends. They found that the Mooney number, shear viscosity and cure rate increased with reclaimed content, while the cure time was independent of the reclaimed content. The property changes of the reclaimed/NR blends were mainly associated with the crosslink precursor or untreated curatives, and the amount of carbon black present in the reclaimed rubber. Sreeja & Kutty  studied the cure characteristics and mechanical properties ofNR/reclaimed rubber blends using EV system. They observed that the scorch time and tensile properties of the blends reduced with the reclaimed loading. It has been widely known that the properties of the vulcanizates are very much dependent on the conditions where the green rubbers are cured, these including cure time and temperature used, design of vulcanizing recipes, as well as the type of curing systems. The last factor is referred to as the methods used for curing the rubber compounds. The most simple curing system used in the rubber industry is direct heating (conventional thermal curing). Many published works have suggested that the duration and mould temperature are the main parameters that control the degree and type of crosslinks to be formed, and these directly affect the properties of the vulcanizates. Microwave curing has increasingly become one of the interesting curing systems in many applications, such as food industries, dried wood systems, concrete curing, and shape-setting of thermosets and rubbers. The main advantages of the microwave cure include faster curing times, improved efficiency of curing, and enhanced mechanical properties of the products . Subjects on the effects of microwave curing on the changes in cured material properties in comparison with those by conventional thermal method are still unclear and open for discussion, since its information are still rare in literature, especially when some secondary materials like reclaimed and carbon black are incorporated. In this work, tire-trade reclaimed rubber were loaded into natural rubber compounds having 60phr of carbon black which were then cured by two different methods, these including conventional thermal and microwave methods. The physical and mechanical properties of the cured rubbers were then examined and compared. Raw materials Experimental The rubbers used in this work were NR (STR20CV) supplied by Tech Bee Hung Co., Ltd. (Bangkok, Thailand) and tire-trade reclaimed rubber (UCD-103 grade) supplied by Union Commercial Development Co., Ltd. (Samutsakorn Thailand). The reclaimed rubber comprised of 24% carbon black, 15% acetone extract and 6% ash. The ratio ofNR:reclaimed rubber used 100:0, 70:30 and 40:60 (%wt). All rubber blends were loaded with 60 phr carbon black (N330), supplied by Thai CarbonBlack Co., Ltd. (BKK, Thailand).